1 MATERIALES PARA EL DESARROLLO SUSTENTABLE Dra. Patricia Eisenberg Coordinadora de la Unidad Técnica Tecnología a de Materiales INTI-Pl Plásticos
2 Bio Polymers or Biobased Polymers Renewable Resource-based Microbial synthesized
4 COMPOSITE MATERIAL FROM COTTON SEED PROTEIN AND NATURAL FIBER
5 Protein Extraction from cottonseed pellets at Pilot Plant Scale (INTI-Cereales) Pellets Production Oil extraction (VICENTIN) -Pressing(90 C) - Hexane extraction (60 C) - Solvent elimination (90 C) - Granulation (pellets)
6 SDP Water Crosslinking agent 30 min,, 30 C 500 rpm ph = 10,TEA 15 min 30 C 500 rpm 15 min 30 C 500 rpm Plastizacer Degasification Filmogenic Solution
7 Reinforced Formie Films Mecanical Properties Maximum Tensile Strength (MPa) % % 36% FNR Formie Formie 36% fiber content produce ~ 750 % increase in MTS & 96% in % elongation lost % Elongation 18 % fiber content produce ~ 460% increase in MTS & 93% in % elongation lost FNR Formie 17,8% Formie 36,3%
8 Reinforced Hemp Films Mecanical Properties Maximum Tensile Strength (MPa) % Elongation % 7 % 22 % FNR Hemp Hemp Hemp FNR FRH7,4 FRH22 FRH45,4 45% fiber content produce ~ 621% increase in MTS & 95% in % elongation lost 22% fiber content produce ~ 320% increase in MTS & 91% in % elongation lost 7% fiber content produce ~ 240% increase in MTS & 90% in % elongation lost
9 Nanocomposites are a new class of materials filled with nanometers size mineral particles instead of conventional scale fillers Professor Amar K. Mohanty, Michigan State University, Copyright 2005
10 Wheat Gluten Protein - Montmorillonite Nanocomposite (MMT-Na Na+) SC gluten O % MMT- Na+ SC gluten 5% MMT- Na+ Tensile Strength (MPa) 6.8 ± 1.5 a 10.6 ± 0.8 b % Strain at Break 63 (20) 45.4 (6) Young Modulus (MPa) 442 (114) 617 (116) Water Vapour Permeability (WVP at 50% RH) left: 0 % MMT-Na+; right: 5% MMT-Na+; SC gluten O % MMT- Na+ SC gluten 5% MMT-Na+ Thickness WVT (µm) (g/s*m*pa) Nanocomposite Guten /Montmorillonite- Na ,75E-11 present 56 % increase in TS 184 1,72E % reduction in WVT
11 Water up take Mass (% ) WG N Water abs WG N Soluble WG Water abs WG Soluble time (min)
12 XRD pattern for WG and WG-MMT MMT-Na (5%) composite Diffractogram showed a similar pattern to that of WG without MMT-Na indicating that sufficient intercalation/exfoliation was achieved in these nanocomposites.
15 XRD pattern for Soy and Soy-MMT MMT-Na composite INTI-Plásticos
16 INTI-Plásticos CIDCA-CONICET 0 % MMT 5 % MMT 10 % MMT x x
17 Nanoclays effects on protein composite films Increase mechanical properties Decrease water sensitivity Decrease water vapour permeability
18 Polycaprolactone Nanocomposites (PCL-MMT) Study of the influence of Montmorillonite structure in the PCL nanocomposite properties Commercial grade poly (ε-caprolactone) FB 100 was supplied by Solvay Chemical (Perstorp caprolactones), mean Molecular Weight >100,000; melting Point 58ºC-60ºC. Clay minerals were CloisiteTM Na+ (native montmorillonite) and "CloisiteTM 30B" (organic modified montmorillonite)(southern Clay Products). Cloisite 30 B is a natural montmorillonite modified with a methyl, tallow, bis-2-hydroxyethyl, quaternary ammonium (Figure 1). The modifier concentration was 90 meq/100g clay. Clay moisture content was < 2 wt. % and its specific gravity was 1.98g/cc. Interlayer spacing d(001) was 1.85 nm.
19 Cloisite 30B
20 COMPOSITE PREPARATION PCL/montmorillonite (PCL-MMT Na and PCl-MMT 30B) were prepared by melt intercalation in Brabender Plasticorder mixing chamber 30 cm3, at 100 C, 90 rpm for 10 min. The collect molten materials were compression-molded into 0,4 mm-tick plates by hot pressing at 100 ºC for 2 min., and then 2 min under 50 bar. The nanocomposites contained 5% of MMT.
21 Analysis of clay dispersion and intercalation/exfoliation in the nanocomposite material. PCL MMT Na a MMT Na 13.4 Å PCL MMT 30B MMT 30B
22 TEM Polycaprolactone Nanocomposites (PCL-MMT) 1 mm= 0.6 µm PCL-MMT Na PCL-MMT 30B
23 Mechanical Properties PCL PCL MMT Na 5% PCL- MMT 30B 5% Young modulus (MPa) Tensile Strength at break (MPa) 36,4 26,6 36,1 Elong.. at break (%) EB (%) TS (MPa) Tensile Strength at Break PCL PCL-MMT Na PCL-MMT 30B Elongation at Break PCL PCL-MMT Na PCL-MMT 30B o difference between tensile strength for PCL and PCL-MMT 30 B, but lower lue was found for PCL-MMT Na. The same trend is observed for the elongation break.these results agree with the intercalation/exfoliation structure for PCL-
24 Comparative Burning Characteristics of Solid Plastics in a Vertical Position The nanocomposite burning behaviour was studied by vertical burning test, adapted from UL 94 The procedure consists of subjecting a set of specimens of identical composition and geometry to a standard test flame for two 10s flame applications. The after flame time is recorded after the first flame application (t1). After the second flame application, the after flame time is recorded (t2). Information is also recorded out whether or not flaming material drips from the specimen and total flame time for a particular specimen set.
25 The different burning characteristics found for PCL- MMT 30 B compare to PCL and PCL-MMT Na could be due to clay intercalated/exfoliated and percolated in the PCL matrix. This interaction provides physical integrity to the material burning, avoiding a configuration in which dripping of flaming material could occur, which constitutes an additional fire propagation to surrounding materials
26 Nanocomposites PCL / PHB /MMT 30 B Preliminary evaluation of the effect of organic modified MMT 30B on one particular composition of PHB/PCL blend, similar to the composition of a commercial PHB/PCL blend, was done. PCL FB 100 was supplied by Solvay Chemical PCL/PHB 40/60 blends and Biocycle (Industrial PHB S.A. (Brazil) nanocomposites (5% MMT-30B) were prepared in Brabender Plasticorder mixer at 170º C/80 rpm/ 10 minutes.
27 Mechanical Properties PHB / PCL Blends Modulus (MPa) PHB/PCL 60:40 PHB/PCL 60: B 5 Biclycle Biclycle + 30B Type Blend A 38 % increase in modulus was observed for the nanocomposite PCL/PHB (40/60)-MMT 30 B. For the commercial polymer Biocycle nanocomposite a 24 % increase in modulus was observed.
28 DMTA of PCL/PHB (40/60) blend and nanocomposite 1,00E+10 PHB/PCL 60:40 PHB/PCL 60:40 /30B :5 1,00E+09 E' (Pa) 1,00E+08 1,00E Temperatura (ºC) MMT 30 B allows the use of this composite blend in temperature range where the PCL/PHB (40/60) blend has already a constant decay in modulus value.
29 SEM PHB/PCL 40/60 blend and PCL/PHB MMT 30 B Without clay 5% MMT 30 B
30 SEM images PCL/PHB 40/60, PCL/PHB40/60 MMT 30 B PCL, PHB PCL disperse phase domain size decreases drastically when nanoclay is incorporated due to the localization of the clay in the interfacial region (TEM)
31 TEM image of PCL/PHB (40/60) blend PCL PHB
32 TEM images PCL/PHB40/60 MMT 30 B MMT 30B PCL MMT 30B PHB PCL PHB
33 PCL/PHB 40/60, PCL/PHB40/60 MMT 30 B and Biocycle nanocomposite SEM images show that the disperse phase domain size decreases drastically when the MMT 30 B is incorporated, in both materials. This behavior is due to the localization of the clay in the interfacial region, as it was confirmed by TEM images. PCL/PHB (40/60) nanocomposite 38 % increase in modulus compare to PCL/PHB (40/60) blend.